DOI 10.1007/s10704-017-0242-y O R I G I NA L PA P E R

**Phase structural ordering kinetics of second-phase**

**formation in the vicinity of a crack**

**C. F. Nigro** **· C. Bjerkén · P. A. T. Olsson**

Received: 13 October 2016 / Accepted: 16 August 2017 © The Author(s) 2017. This article is an open access publication

**Abstract** The formation of a second phase in
pres-ence of a crack in a crystalline material is modelled and
studied for different prevailing conditions in order to
*predict and a posteriori prevent failure, e.g. by delayed*
hydride cracking. To this end, the phase field
formu-lation of Ginzburg–Landau is selected to describe the
phase transformation, and simulations using the finite
volume method are performed for a wide range of
mate-rial properties. A sixth order Landau potential for a
single structural order parameter is adopted because it
allows the modeling of both first and second order
tran-sitions and its corresponding phase diagram can be
out-lined analytically. The elastic stress field induced by the
crack is found to cause a space-dependent shift in the
transition temperature, which promotes a second-phase
precipitation in vicinity of the crack tip. The
spatio-temporal evolution during nucleation and growth is
successfully monitored for different combinations of
material properties and applied loads. Results for the
second-phase shape and size evolution are presented
and discussed for a number of selected characteristic
cases. The numerical results at steady state are
com-pared to mean-field equilibrium solutions and a good
agreement is achieved. For materials applicable to the
model, the results can be used to predict the evolution of
an eventual second-phase formation through a

dimen-C. F. Nigro (

### B

)· C. Bjerkén · P. A. T. Olsson Materials Science and Applied Mathematics, Malmö University, 205 06 Malmö, Sweden e-mail: claudio.nigro@mah.comsionless phase transformation in the crack-tip vicinity for given conditions.

**Keywords Phase transformation**· Mode I crack ·
Phase field method· Ginzburg–Landau formulation ·
Precipitation kinetics

**1 Introduction**

Most metallic materials experience some type of inter-action with their surrounding environment, which often results in changes in the material morphology that may induce deterioration of their mechanical and physi-cal properties. For many practiphysi-cal applications such changes may derogate a material function and its use-fulness, which may eventually lead to failure. If stresses are applied to a structure subjected to a corrosive envi-ronment, cracks that would not occur in the absence of one of these two controlling conditions will appear, even for virtually inert material. Thus, the combination of these factors may lead to failure, which is commonly referred to as stress corrosion cracking (Jones 1992).

Hydrogen embrittlement (HE) can be considered to be a type of stress corrosion, since it commonly con-cerns a ductile metal undergoing a brittle fracture as a result of the combination of applied stresses and a corrosive environment. HE can also occur in mechan-ically loaded materials that already contain hydrogen emanating from either the manufacturing process or from earlier exposure to hydrogen. For some cases of

HE, hydride formation plays a central role in the detori-ation process. A hydride is a brittle non-metallic phase that may cause the embrittlement of metallic materi-als such as titanium- and zirconium-based alloys and reduce their load bearing capabilities (Coleman and Hardie 1966;Coleman et al. 2009;Chen et al. 2004; Luo et al. 2006). For metal based components exposed to hydrogen-rich environments, such as fuel cladding materials in nuclear power reactors or components in rocket engines, there is an impending risk of hydrides forming, which could lead to the so called delayed hydride cracking (DHC). This is a subcritical crack growth mechanism (Coleman et al. 2009;Singh et al. 2004;Coleman 2007;Northwood and Kosasih 1983) that can severely reduce the component life-time and jeopardize its integrity.

Hydride formation occurs as a result of a
combi-nation of complex mechanisms, including for instance
simultaneous hydrogen diffusion, hydride precipitation
and material deformation (Varias and Massih 2002).
For some metals, including zirconium and titanium,
such formation has been specifically observed in the
vicinity of stress concentrators, following the increased
hydrogen transport toward regions of high hydrostatic
stresses (Birnbaum 1976; Takano and Suzuki 1974;
Grossbeck and Birnbaum 1977;Shih et al. 1988;Cann
and Sexton 1980). It is also known that the
transfor-mation is not only driven by changes of
concentra-tion of species, such impurities and alloying elements,
*but mechanical stresses can per se promote the *
pre-cipitation of a second phase (Birnbaum 1984; Allen
1978;Varias and Massih 2002). This type of
transfor-mation can be beneficial for instance for certain ceramic
materials, which may experience an increase in
frac-ture toughness following the transformation. For such
cases, the crack propagation may be impeded following
the transformation of metastable phase particles into
stable particles with increased volume at the crack tip
(Hutchinson 1989;Evans and Cannon 1986). Thus, the
resulting transformation-induced compressive stresses
in front of the crack-tip may obstruct its opening and,
consequently, limit the crack growth. However, for the
case of transition metals and hydrogen, such
benefi-cial transformation is rarely observed. In fact, for the
hydride forming materials the effect is rather the
oppo-site, leading to embrittlement and reduction of the
frac-ture toughness.

Over the years, numerous models have been devel-oped to describe the formation of a second phase

at a flaw tip in a variety of crystalline materials (Varias and Massih 2002; Deschamps and Bréchet 1998;Gómez-Ramírez and Pound 1973;Boulbitch and Korzhenevskii 2016; Léonard and Desai 1998; Hin et al. 2008;Massih 2011a;Bjerkén and Massih 2014; Jernkvist and Massih 2014; Jernkvist 2014). Among those are the models resting on the phase-field approach based on Ginzburg–Landau theory, see e.g.Provatas and Elder (2010). Such modeling has found many applications, especially in the areas of magnetic field theory where it has been found useful for providing predictive models (Cyrot 1973; Berger 2005; Barba-Ortega et al. 2009;Cao et al. 2013; Gonçalves et al. 2014). But more importantly for the present applica-tion it has also proven to be an efficient methodology to model and predict microstructure evolution in mate-rials. The review paper byChen(2002) and the refer-ences therein give a thorough account of applications for which phase-field modeling has been successfully used to predict the microstructural evolution. For phase field theory applied to solid material microstructure modeling order parameters are used to describe the evo-lution of a material state (Desai and Kapral 2009). Typ-ically, two different order parameters may be identified to describe different type of phase transformations: the non-conserved structural order parameter correspond-ing to a diffusionless-type transformation and the con-served composition order parameter which represents a diffusional transformation. With this in mind, Hohen-berg and Halperin(1977) defined three types of models based on the use of these order parameters individu-ally (model A and B, respectively) and their coupling (model C).

In the material, the solid solution may be defined as a disordered material state and crystal structures with a lower degree of symmetry are considered ordered. Under stress field conditions, such as stresses induced by the presence of flaws, the evolution of the order parameters are used to model a second-phase forma-tion. One such study was reported byMassih(2011a), who presented a general set-up with coupled conserved and non-conserved field variables in the presence of cracks and dislocations in an elastic solid. Further, in a paper byBoulbitch and Korzhenevskii(2016), a non-conserved order parameter is used to study quasi-static phase transformation in the process zone of a propa-gating crack. These works constitute a suitable base reference to study the second-phase formation in pres-ence of a crack. In the present paper, the effect of stress

concentration in the presence of a crack on the second-phase formation kinetics in crystalline materials is modeled. This work is an extension of the Massih’s and Bjerkén’s works (Bjerkén and Massih 2014; Mas-sih 2011b), where precipitation kinetics at dislocations is studied by using a scalar non-conserved order param-eter (Model A), accounting for microstructural reorder-ing. The time-dependent Ginzburg–Landau (TDGL) equation is solved numerically to capture the differ-ent spatio-temporal state changes of the material in the vicinity of the crack tip. This is achieved by assess-ing the spatio-temporal fluctuations of the structural order parameter for different sets of material parame-ters, loads and phenomenological coefficients, making of this paper a full parametrical study, usually undone in the literature. The driving force of this equation, which gives the rate of change the structural order parameter, is the functional derivative of the total free energy with respect to the non-conserved order param-eter (Provatas and Elder 2010). To include the effect of the crack to the modeling, a mechanical equilib-rium condition is added to the free energy formulation for the system at hand. The mechanical equilibrium is solved analytically reducing the number of equations to be solved to one, the TDGL equation, as inBoulbitch and Korzhenevskii(2016). To this end, a small pertur-bation from a stressed reference configuration under known stress conditions due to the presence of the crack is assumed. A sixth-order Landau potential energy is incorporated in the structural free energy of the system in order to model first and second order transitions. Moreover, the total free energy of the system takes into account a coupling between the dilatation of the second phase and the order parameter (Boulbitch and Tolédano 1998). The effect of hydrogen concentration is not con-sidered in the model.

The paper is organized as follows: first, the model employed to study the formation of the second phase in presence of the crack is described in Sect.2. This description is followed by a theoretical steady-state analysis, accompanied by a phase diagram, in Sect.3. Thereafter, the methodology for the numerical simu-lations is presented in Sect.4. The following section, Sect. 5, demonstrates the results obtained for differ-ent cases and parameters which contains comparisons between theoretical steady-state and long-time numer-ical data and the influence of the interface energy on the solutions. Finally, in Sect.6, the findings are sum-marized and the conclusions are stated.

**2 Model description**

In the Ginzburg–Landau formalism, a parameter field*η*
is defined as a scalar function that represents the order
of the crystal structure and characterizes the presence of
two concurrently prevailing phases. The order
param-eter depends on time and space and defines the
mor-phology such that the high-temperature solid solution
that constitutes the initial phase corresponds to*η = 0,*
whereas the transformed second-phase precipitates are
represented by*η = 0. For such systems the total free*
energy,*F , can be expressed as*

*F = Fst+ Fel+ Fi nt,* (1)

where*Fst*stands for the structural free energy,*Fel*the

elastic-strain energy and*Fi nt* is the striction energy,

which represents the interaction between the structure
order parameter and the strain field (Ohta 1990;Massih
2011b). Each individual contribution to the free energy
in (1) can be represented by an integral over the system
*volume, V . The structural free energy is expressed by:*
*Fst* =

* _{g}*
2

*(∇η)*

2_{+ Ψ (η)}

* dV.* (2)

in which the term 1_{2}*g(∇η)*2 accounts for a spatial
dependence of the order parameter and the existence of
interfaces within an equilibrium inhomogeneous
sys-tem (Desai and Kapral 2009). The positive coefficient
*g takes part in the surface energy by multiplying the*
gradient in order parameter which only varies
signif-icantly at interfaces where a change of order occurs
(Provatas and Elder 2010). The second term*Ψ (η) is*
a phenomenological contribution to the free energy
that was introduced byLandau and Lifshitz(1980) as
the Landau potential and coincides with the bulk free
density. In the present work we assume a sixth order
description, expressed in the format

*Ψ (η) =* 1
2*α0η*
2_{+} 1
4*β0η*
4_{+}1
6*γ η*
6* _{.}*
(3)
where

*α0, β0*and

*γ are named Landau coefficients in*the present paper. The coefficient

*α0*displays a lin-ear variation with the material temperature as

*α0*=

*[T −Tc*0

*], where the parameter a is assumed to be a*

*pos-itive constant and T is the material temperature and the*
*parameter Tc*0 is the transition temperature for a defect

free crystal (Provatas and Elder 2010). The definition
of *α0* is the result of an assumption of the Landau’s
theory which states that*α0changes sign at Tc*0 (

temperature independent when the material
*tempera-ture is sufficiently close to Tc*0 (Cowley 1980;Massih

2011a). Additionally, to ensure stability of the system
the condition*γ > 0 is required whenever β0< 0. The*
elastic strain energy is expressed as

*Fel* =
*M*
2
*i j*+
*K*
*2 M* −
1
*d*
2
*ll*
* dV,* (4)

*where K and M are the bulk and the shear *
*mod-uli respectively. The parameter d represents the space*
dimensionality of the considered system, while the
strain tensor is defined within the small perturbations
hypothesis, i.e. *i j* = 1_{2}*(∂uj/∂xi* *+ ∂ui/∂xj). The*

striction energy is written on the format
*Fi nt* =

*−ξ η*2_{∇ · u dV.}_{(5)}

that represents the interaction between the order
**param-eter and the displacement vector field u** *= ui*. This

contribution is characterized by the assumed
posi-tive constant *ξ, also known as the striction factor.*
The striction factor is related to e.g. lattice mismatch
and volume changes between phases, and represents
the stress derived from the stress-free strain, i.e. the
stress-free expansion. The quantity**∇ · u represents the**
strain resulting from the stress induced by the crack
(Eshelby 1957). The dilatational effects are assumed
to be isotropic and are taken into account in the
inter-face between second phase and solid solution, and in
the second phase.

Based on Eqs. (2), (4) and (5), the total free energy of
the system can be rewritten in a more compact notation
*F =*
* ϕ(η(r, t), u(r, t))dV* (6)
with

**ϕ(η(r, t), u(r, t)) =***g*2

*(∇η)*2

_{+ Ψ (η)}*+ M*2

*i j*+

*K*

*2 M*− 1

*d*2

*ll*

*− ξ η*2

*(7) such that*

_{∇ · u.}*ϕ is the volume specific energy density of the*system. Thus, mechanical equilibrium for the system, which is assumed to exist at all time, requires that

*∂σi j*
*∂xj* = −
*δF*
*δui* =
*∂*
*∂xj*
*∂ϕ*
*∂i j*
*= Qi* (8)

where*σi j* *is the stress tensor and Qi* denotes a body

force field, which is induced by the presence of an elas-tic defect in the solid (Massih 2011b). In the present

work the considered flaw is a crack. Equation (8) can be further reduced to

*M*∇2**u*** + (Λ − M)∇∇ · u − ξ∇η*2

*(9) where*

**= M f(r)***Λ = K + 2M(1 − d*−1

*of space that describes the strain field due to the crack (Massih 2011a). By solving Eq. (9) with respect to the elastic strain field, as proposed inMassih(2011b) it can be substituted into Eq. (7), which leads to the total free energy of the system being transformed to a functional described solely by the order parameter*

**) and f(r) is a function**

**η(t, r):***F [η] =*

*g*2

*(∇η)*2

_{+}1 2

*α η*2 +1 4

*β η*4

_{+}1 6

*γ η*6

_{d r}_{(10)}

Following this rewrite, based on the assumptions of
lin-ear elastic fracture mechanics under plane strain
condi-tions and mechanical equilibrium, the modified Landau
coefficients for the quadratic and quartic terms (i.e.*α*
and*β in Eq. (*3), respectively) are given by

*α ≡ |α0|*
sgn*(α0) −*
*r0*
*r* cos
*θ*
2
(11)
and
*β = β0*−2ξ2
*Λ* *,* (12)
where
*r0*≡ 1
2*π*
2*ξ KI*
*|α0| (Λ − M)*
2
*.* (13)

is considered as a local characteristic length related to
*the presence of the crack and KI* is the mode I stress

intensity factor. It should be noted that for a defect-free
crystal,*α = α0*and*β = β0.*

The considered geometry of the crack is described by polar coordinates with the origin placed at the crack tip, as shown in Fig.1. Under plane strain, the crack may be seen as semi-infinite, i.e. its thickness is infinite in the out-of-plane direction.

Depending on the stress field induced by the crack,
the solubility limit may vary at different positions
rela-tive to the crack tip. In order to capture such a behaviour,
*α [in Eq. (*11)] is expressed as

*α = a [T − Tc(r, θ)] ,* (14)
where
*Tc(r, θ) ≡ Tc*0+
2*ξ KI*
*a(Λ − M)*
cos(θ/2)_{√}
2*π r* *.* (15)

**Fig. 1 Geometry of the crack. The coordinates are represented**

*by the polar coordinates r andθ*

*The parameter Tc(r, θ) defined above is the transition*

temperature for a crystal containing a crack. Thus,
the initial phase of a defect-free material is stable for
*T* *> Tc*0, while that of a cracked material requires

*T* *> max(Tc, Tc*0*), which implies α > 0. *

Conse-quently, a secondary phase will form in the region of
the material where these conditions are not met.
Like-wise, owing to their influence on*β, an increase of ξ and*
a decrease in*Λ contribute to the formation and growth*
of a second phase.

The evolution of the non-conserved structural order parameter is determined by the employment of the TDGL, which corresponds to a diffusionless phase transformation model (Hohenberg and Halperin 1977), i.e.,

*∂η*
*∂t* *= −Γ*

*δF*

*δη.* (16)

where*Γ is the kinetic coefficient that represents the*
interface boundary mobility. By substituting the total
free energy term of Eq. (10) into (16), the
govern-ing equation for the spatio-temporal order evolution
becomes
1
*Γ*
*∂η*
*∂t* *= g∇*
2* _{η −}_{α η + β η}*3

*5*

_{+ γ η}*(17) For practicality in the modeling and the subsequent analyses, a parameter change to obtain a dimensionless equation is made:*

_{.}*η =*

*|α0|/|β| Φ, xi*=

*g/|α0| ˜xi, r =*

*g/|α0| ρ,*

*r0*=

*g/|α0| ρ0*

*and t*

*= τ/ (|α*0

*| Γ ) .*

Following this manipulation, via the dimensionless
analogues of Eqs. (16) and (17), the relation describing
the transformed order parameter,*Φ, is given by*

*∂Φ*
*∂τ* = ˜∇
2_{Φ −}*AΦ + sgn(β) Φ*3*+ κ Φ*5
(18)
*where A* =
sgn*(α0) −**ρ*0
*ρ* cos*θ*2
, ˜∇ is the
dimen-sionless gradient operator for the rescaled coordinates

*˜xi* *= ( ˜x, ˜y) and κ = γ |α0|/β*2.

To gain insight behind the second phase
nucle-ation around a crack tip, in the present study we solve
Eq. (18) for different sign combinations of*α0* and*β.*
This aims to investigate the importance of
tempera-ture induced solubility variation for different
materi-als, while the interaction between displacement field
and order parameter are varied.

**3 Steady-state analysis**

As an initial study, we analyze the steady-state
solu-tion of Eq. (18). This corresponds to the long-time
limit, at which the system does not evolve further and
no additional transformations occur. This implies that
*∂η/∂t = 0. Here, the Laplacian term is neglected. The*
physical interpretation of this simplification is that the
value of the order parameter in a material point is not
affected by the surrounding points. The neglect of the
Laplacian term is also expected to induce the
appear-ance of discontinuities of the function*Φ(x, y) at the*
crack tip and at the transition between zero and
non-zero values of the order parameter. Thus, Eq. (18) is
simplified as

¯

*Φ*
*A+ sgn(β) ¯Φ*2*+ κ ¯Φ*4

*= 0,* (19)

where ¯*Φ is the order parameter of such a steady-state*
system containing a crack. Depending on the parameter
set, the solutions to (19), which either minimize or
max-imize the total free energy of the system in steady state,
can be found analytically. The real analytical solutions
of Eq. (19) may be expressed as:

⎧
⎪
⎨
⎪
⎩
¯
*Φ0*= 0
¯
*Φ*2
±= *−sgn(β) ±*
√
1*− 4 A κ*
2*κ* *.*
(20)
(21)
The stability condition*γ > 0 ensures positive values*
of*κ for any couple {α0, β}, and if ¯Φ exists, the *
solu-tions always correspond to local extrema of the
modi-fied Landau potential. Thus, the existence of non-zero

**Fig.** **2 Phase** diagram presenting the length ratio
*ρ /**ρ*0cos2*(θ/2)* versus *κ sgn(β) for α*0 *> 0. The star*

(*) indicates that the phase is metastable, and the disorded
phase is denoted I, while the ordered is denoted II. The vertical
*asymptotes of the curves given by A* = _{4}1_{κ}*and A*= _{16}3* _{κ}* are

*indicated with dashed lines*

solutions to Eq. (19) depend on the signs of*α0*and*β*
and the value of*κ. The deduction of stability limits and*
phase transition characteristics for different values of
*{α0, β} are given in “Appendix”, and is summarized*
for*α0> 0 in Fig.*2as a phase diagram.

When*α0* *< 0, the parameter A is always negative.*
*This means that the transition temperature Tc*becomes

*higher than the material temperature T , regardless of*
the distance from the crack. Thus, the whole
mate-rial is expected to transform into the second phase. If
instead*α0* *> 0, a second-phase region may form in*
the proximity of the crack tip with the size of the zone
depending on the value of*κ sgn(β). For this case the*
transition temperature is higher than the material
tem-perature only locally, which explains the limited local
transformation. For*β > 0, only second order *
transi-tions between the phases may take place as the stability
*lines of the phases coincides (at A*= 0), regardless of
the value of*κ. For negative β, the regions of stability of*
the individual phases overlap, where a phase either may
be stable or metastable. The stability limits for phase I
*( A= 0) and II (A = 1/4κ) are indicated in the figure.*
*Between these limits the transition line A*= _{16}3* _{κ}*can be
identified, which represents a situation at which both
phases are equally stable and only first order transitions
are expected.

It can be seen that in immediate proximity to the
crack tip (i.e.*ρ/[ρ0*cos2*(θ/2)] < 1), the stress *
con-centration induces a transformation from solid solution
into the second phase. Further away from the crack, the
situation may vary depending on the sign of*β and the*
value of*κ. As κ sgn(β) < −3/16, the material can be*
in four different states, and sorting them with
increas-ing distance from the crack tip, they correspond to:

– a pure second-phase area, II,

– an area with second phase and metastable solid solution, I* + II,

– an area with solid solution with metastable second phase, I + II*, and

– a pure solid solution, I.

For−_{16}3 *< κ sgn(β) < 0, it is found that the whole*
material is supposed to be transformed into second
phase (II) with the possible presence of metastable solid
solution away from the crack tip (ρ/[ρ0cos2*(θ/2)] >*
1). Finally, when*κ sgn(β) > 0 no metastable state*
can exist but a confined pure second-phase region
should develop in the region close to the crack tip (i.e.
*ρ/[ρ0* cos2*(θ/2)] < 1).*

**4 Numerical method**

To numerically solve the TDGL equation, presented
in Sect. 2, we use the open-source partial
differ-ential equation solver package FiPy (Guyer et al.
2009), which is based on a standard finite volume
approach. For the modeling, the 2d-domain illustrated
in Fig.1is discretized using a square mesh consisting
of 1000× 1000 equally-sized square elements with the
dimensionless side length corresponding to*Δ˜l = 0.2.*
This setup, combined with a LU-factorization solution
scheme, was found to yield well converged results and
the system is large enough such that the boundary
con-ditions do not affect the results. The size of the time step
is deduced from a convergence study, which revealed
that a time step*Δτ = 0.1 is sufficient to ensure a stable*
solution.

At the boundary, the gradient of*Φ is prescribed to*
be perpendicular to the boundary such that**∇Φ ·n = 0,****where n is a unit vector perpendicular to the boundary.**
As initial condition the order parameter,*Φi ni t* was

randomly set throughout the entire domain, with values
in the range[5 × 10−5*, 1 × 10*−4].

**5 Results and discussion**

In this section, the spatio-temporal evolution of the
dimensionless order parameter *Φ is presented. *
Par-ticular emphasis is on modeling and elucidating the
material transformation for varying signs of*α0*and*β*
and the varying value of*κ. These combinations *
rep-resent different characteristic locations in the phase
diagram illustrated in Fig.2. Thereafter, the
numer-ically obtained steady-state results are discussed with
reference to the analytical mean-field solutions given in
Sect.3. Moreover, the width of inherent smooth
inter-face is discussed, and finally, the influence of material
stiffness and strength of interaction between strain field
and order parameter are investigated.

5.1 Temperature higher than bulk transition
*temperature: T* *> Tc*0

*If the temperature T* *> Tc*0, no phase transition is

expected in an un-cracked material, and implies that
*α = α0> 0. The introduction of a loaded crack results*
in a shift of*α, see Eqs. (*11), (14), whose magnitude
depends on the position relative to the crack tip. In
gen-eral, the closer to the crack tip, the higher the stress,
and the larger the shift, which inevitably implies that
the driving force for the phase transformation is larger.
With a sixth order potential, both second and first
order transitions can be modeled. According to the
phase diagram in Fig. 2, both first order transitions
can occur in a homogeneous material when*κsgn(β) <*
*−3/16. Thus, it could be of interest to investigate of the*
evolution of a second phase in the presence of a loaded
crack for a corresponding case; here*κsgn(β) = −1*
is chosen. The results from the numerical simulation
of the evolution of the order parameter are presented
in Fig.3a–c. From this figure sequence, it is seen that
a ”kidney”-shaped zone with*Φ = 0 is developing in*
the vicinity of the crack tip, which is an indication of
precipitation of a second phase. To further illustrate
the space dependence of*Φ during the evolution, the*
profile of the cross-section of the*Φ-surface along the*
*˜x-axis ( ˜y = 0) is given at different instants in Fig.*3d.
Two main stages in the order parameter evolution may
be identified: initially a relatively sharp peak emerges
close to the crack tip where the material locally
trans-forms, thereafter the transformed region expands in
*space until a steady state (ss) is reached. The *

**succes-Fig. 3 a–c Evolution of the dimensionless order parameter***Φ =*

*Φ(x, y) for the case with α*0*> 0 and κ sgn(β) = −1 at different*

**instants; d Profiles of***Φ( ˜x, ˜y = 0) between τ = 0 and τ = 50.*
*The arrow illustrates the evolution direction with time for˜x > 0*

**Fig. 3 continued**

sive increase of the order peak value*Φpeak* is

evalu-ated and its temporal evolution is presented in Fig.4a
(cyan line). During the expansion stage, it is found that
the phase interface moves in the positive *˜x-direction*
with a seemingly constant slope, see Fig.3d. Because
the model inherently relies on the assumption that the
interface between the two phases is smooth, no exact
boundary can be distinguished. Thus, to quantify the
expansion of the second phase, we monitor the width
*˜w of the Φ-profile illustrated in Fig.*3d and defined *˜w*
as the distance from the origin to the point along
posi-tive*˜x at which Φ = 0.01. The results in Fig.*4b (cyan
line) reveal that *˜w converges following an asymptote,*
implying that there is a steady-state size.

Other cases where *κ sgn(β) < −3/16 are also*
studied. Similar evolution patterns are obtained as for
*κ sgn(β) = −1, i.e. an initial order parameter peak*
rises followed by a limited space expansion. Yet, the
evolution have other characteristic values, e.g. the
max-imum values of*Φpeak* and *˜w, respectively, vary, see*

Fig.4.

To investigate the span*−3/16 < κ sgn(β) < 0,*
the evolution of*Φ is calculated for the specific case*
of *κ sgn(β) = −1/9, which is deemed *
representa-tive for the interval. The evolution of the*Φ-profile is*
presented in Fig.5. Initially, the evolution pattern is
similar to that observed for the previously considered
parameter sets. However, as the precipitate continues
to grow, it expands with seemingly constant speed with
no tendency to slow down in order to eventually reach a
steady state. According to the phase diagram in Fig.2,

**Fig. 4 Evolution of a the peak value of the order parameter**

*Φpeak***, and b the shape width***w of the Φ-profile where Φ = 0.01*

for*θ = 0. (α*0*> 0 in all cases.)*

no matrix phase (I) should exist at steady-state in a
homogeneous material when*α > 0, thus making the*
proposed scenario plausible.

Additionally, the situation for positive values of*β*
is considered, which is motivated by the phase
dia-gram that only predicts second order transition
regard-less of value of*κ, cf. the limit A = 0 in Fig.*2.
Fig-ure6shows the evolution of the*Φ-profile for κ = 1,*
whose behavior somewhat resembles that of the case
for*κ sgn(β) = −1 (Fig.*3d) with a fast initial increase
of *Φ close to the crack tip. However, the *
broaden-ing is accompanied with a gradually decreasbroaden-ing slope
of the order parameter in the interface proximity, as
opposed to the relatively constant slope observed for
*κ sgn(β) = −1. Simulations with three different values*
of*κ are performed, and the evolution of Φpeak*and *˜w*

**Fig. 5 Evolution of***Φ(x, y = 0) for α*0*> 0, κsgn(β) = −1/9.*

Profiles are shown for*τ = 0 to τ = 50*

**Fig. 6 Evolution of***Φ(˜, ˜y = 0) for α*0*> 0, β > 0 and κ = 1.*

Profiles are shown for*τ = 0 to τ = 50*

for theses cases are included in Fig.4. Neglecting small
numerical variations, the evolution of *˜w is found *
inde-pendent of*κ, i.e. the precipitation shape and growth*
rate are expected to be similar for all cases such that
*β > 0.*

5.2 Temperature lower than bulk transition
*temperature: T* *< Tc*0

To further extend the investigation, modeling of the
situation for which the material temperature is lower
than the bulk transition temperature is performed, i.e.
*T* *< Tc*0 corresponding to*α0< 0. Based on Eqs. (*11)

and (14), it can be shown that for the situation at

hand*α ≤ 0 and T < Tc* must prevail everywhere in

the domain. An example of the evolution of the order
parameter is monitored in Fig.7at different times and
Fig.8illustrates the evolution of the*Φ-profile along*
the *˜x-axis. For the stated conditions, the order *
param-eter*Φ increases in the whole computational cell, i.e.*
the whole material, but its value is higher in the
crack-tip neighborhood where a stress concentration resides.
Similar to the considered situations in the previous
sec-tion, the order parameter displays a peak in the vicinity
of the crack tip, which early on reaches a maximum
value, while a slower transformation is taking place
away from the crack tip.

5.3 Comparisons of evolution characteristics

In order to quantitatively describe the evolution
behav-ior, some characteristics measurements are defined:
*Φmax* denotes the maximum value of*Φpeak, τmp* the

time to reach this value, *˜wss* steady-state width, and

*τ95%ss* required for the system to reach 95% of *˜wss*.

Results for the presented cases are summarized in Table1.

For the situation where*α0> 0, three different types*
of evolution patterns are obtained relating to different
intervals of*κ sgn(β): β > 0, β < 0 ∧ κ > 3/16 and*
*β < 0 ∧ κ < 3/16, respectively. Results from the*
simulations of the corresponding cases are presented
in the following paragraphs, and in the last paragraph
results for*α0< 0 are discussed.*

For all investigated cases where*α0> 0 and β < 0,*
it is found that *Φmax, ˜wss* and*τ95%ss* decrease with

increasing *κ, see Table* 1. In contrast, the time *τmp*

that characterizes the initial stage of the precipitation is
approximately the same (≈5) and not exceeding 20%
of *τ95%ss* for any of the considered cases. The latter
observations are also true for *β > 0. Further, larger*
*Φmax* are reached for negative*β than for positive β*

with same value of*κ.*

It is also found that in cases where *κ sgn(β) <*
*−3/16, wss*increases with increasing*κ sgn(β). It can*

be deduced that there is an approximate linear relation
between the two with dw*ss/dτ95%ss* *≈ ρ0/50. *

How-ever if*β > 0, all choices of κ result in similar values*
of the final width*wss*and the time to reach 95% of*wss*,

respectively. Thus, as been mentioned earlier, the
pre-cipitation process is not influenced by the value of*κ,*
and it can be concluded that a Landau potential of lower

**Fig. 7 Evolution of the dimensionless order parameter***Φ =*

*Φ(x, y) for the case with α*0 *< 0, κsgn(β) < 0 at different*

instants

**Fig. 7 continued**

**Fig. 8 Evolution of***Φ( ˜x, ˜y = 0) for α*0*< 0, κ sgn(β) = 1 from*
*τ = 0 to τ = 50*

order than what is used in this study may be sufficient
to simulate the evolution if*β > 0.*

The characteristic values for two studied cases for
which*α0< 0 are also given in Table*1. The maximum
peak value*Φmax* is found to be larger for negative*β*

than for positive*β for the same value of κ, in line what*
is found for positive*α0. The time to reach this *
max-imum,*τmp*, is approximately equal in both cases, but

about half the time for cases with *α0* *> 0. That the*
evolution process is faster is expected, since the whole
material is quenched and the contribution from stress
concentration to the driving force for phase
transfor-mation is added on top.

**Table 1 Summary of the characteristic values {***Φmax*,*τmp*, *˜wss*and*τ95%ss*} for different combinations of*κ sgn(β) and α*0
*α*0*> 0*
*κ sgn(β)* −4 −2 −1 *−1/4* *−1/9*
*Φmax* 1.12 1.37 1.69 2.70 3.66
*τmp* 4.6 4.6 4.6 4.6 4.4
*˜wss/ρ*0 1.55 1.67 1.92 * −
*τ95%ss* 36.5 40.5 56.0 * −
*α*0*> 0*
*κ sgn(β)* 1 2 4
*Φmax* 1.29 1.13 0.977
*τmp* 4.9 4.8 4.7
*˜wss/ρ*0 1.40 1.39 1.38
*τ95%ss* 28.5 29.5 29.0
*α*0*< 0*
*κ sgn(β)* −1 1
*Φmax* 1.84 1.50
*τmp* 2.3 2.4
*˜wss/ρ*0 − −
*τ95%ss* 10.9 11.7

* Values are not obtained within the calculation time limit 5.4 Comparison with analytic local steady-state

solutions

Here, the numerical results are compared with the ana-lytically deduced local steady-state solutions that are presented in Sect.3, which from now on is referred to as the analytical solutions. This aims at investigating the possibilities and limitations of using these analyti-cal results to predict the evolution pattern for different configurations.

In the analytical study, the Laplacian term in Eq. (18)
is neglected, roughly implying that the solution in each
point in space is unaware of its neighbors. The
Lapla-cian term not only governs the smoothening of the
inter-face between disordered matrix and second phase, but
it also affects the peak shape of the*Φ-profile. In *
addi-tion, it influences the non-zero values of*Φ along the*
crack surfaces.

Figure9a presents the numerically steady-state and
analytical solutions for the case with *α0* *< 0 and*
*κ sgn(β) = 1, where it is found that the curves match*
very well. However, an exception is found very close to
the crack tip where the analytical solution goes to
infin-ity and the effect of the interface energy on the

numer-ical results is pronounced. The same observations can
be done for all studied cases for which*α0* *< 0 and,*
*α0> 0 with −3/16 < κ sgn(β) < 0.*

In Fig. 9b, steady-state profiles for the case with
*α0* *> 0 and κ sgn(β) = −1 are displayed. A match*
is found between the numerical and analytical results
although differences subsist in the direct vicinity of the
crack tip and at the interface between second phase and
solid solution. The location corresponding to the
sta-bility limits of phase I and II are included, as well as the
transition line between region I*+ II and I + II* given
by the phase diagram in Fig.2. It can be seen that the
smooth interface is located about the line that indicates
the first order transition between globally stable phases.
Similar observations can be done for all studied cases
for which*α0> 0 with κ sgn(β) < −3/16 and α0> 0*
with*β > 0. In the latter case however, the smooth*
interface is approximately centered at *˜x = ρ0, which*
corresponds to the second order transition location for
the analytical solution.

The strong resemblances of the curve appearance indicate the numerical steady-state shape and approx-imate size of the second phase can be predicted by using the analytic local steady-state solutions for all

*˜x/ρ*

0
-1 0 1 2 3
### Φ

0 1 2 3 4 Numerical Analytical**(a)**

*˜x/ρ*0 -1 0 1 2 3 Φ 0 0.5 1 1.5 2 2.5 3 3.5 4 Numerical Analytical II I+II* I I*+II

**(b)**

**Fig. 9 Comparison between analytical and numerical **

compu-tations for spatial variation*( ˜x, ˜y = 0) of order parameter in a*
**steady state for a***α*0* < 0 and κ sgn(β) = 1 and for b α*0

*> 0*

and*κ sgn(β) = −1*

cases. However, the assumption that transformation
takes place wherever*Φ = 0 is disputable since that*
numerical solution renders a larger precipitate than
the analytical solution is considered, see e.g. Fig.9b.
Indeed, the numerical result display an interface with
a certain thickness whereas it is sharp in the analytical
solution. The intersection between the curves ahead
the crack tip in Fig. 9b corresponds to an apparent
inflexion point of the interface profile obtained
numer-ically, and the same observation is made for all cases
where*α0> 0 and κ sgn(β) < −3/16. The smoothness*
of the interface depends on the interface energy and
thus cannot directly be predicted from the analytical

solution. Additionally, the steady-state solutions dis-play possible metastable phases. The stability analysis was performed only in a point wise way. However, the metastable phases might not appear if the total energy of the system and the temporal evolution of the space-dependent field are considered.

5.5 Influence of stresses on interface width

To explore the influence of the crack induced stress field
on the characteristics of the diffuse interface, its width
*λ is measured for different values of the gradient energy*
*coefficient g in Eq. (*2). For a phase boundary with an
interface profile that is symmetric in the radial
direc-tion,*λ is proportional to (g/ΔΨ )*1*/2*, see e.g.Moelans
et al.(2008),Provatas and Elder(2010), where*ΔΨ is*
the bulk energy barrier for phase transition, as
illus-trated in Fig.12in “Appendix”. Further, the width*λ*
is often defined as the distance between two positions
for which*Φ = L1Φ0* and*Φ = L2Φ0, see Fig.*10,
where*Φ0*is the maximum value of*Φ. For example,*
the limits 0.1 and 0.9 could be chosen to characterize
the interface width. In present study, all results are
pre-sented using a dimensionless length obtained by scaling
with√*|α0|/g. In case of a symmetric interface, then a*
dimensionless interface width ˜*λ would be independent*
*of g.*

In this study, the investigation of how *λ depends*
*on g in the presence of the loaded crack is limited to*
a single case: *α0* *> 0, β < 0 and κ = 1 at steady*
state. In Fig.9numerical result*(g = 0) and the *
ana-lytical solution*(g = 0) are compared for the *

*consid-x*

### Φ

### /Φ

0 0 1*λ*

*L*

_{1}*L*

*2*

0 0.05 0.1 0.15 0.2 0.25 0.3
*g*1/2
0
0.1
0.2
0.3
0.4
*λ/*
*C* 1
*λ=C*_{1}*(g*1/2*+ C*_{2})
lim 5-95 %
lim 10-90 %
lim 20-80 %
lim 30-70 %

**Fig. 11 Interface width***λ versus g*1*/2*for different limits defining
the width. A linear fit of the results is included

ered case. This comparison reveals that the analytical
solution is discontinuous at the transition point, and
*ΔΦ is taken as the difference in ¯Φ at this location.*
Different limits couples *(L1, L2) are considered for*
*g* *= {1, 5, 7, 10, 50, 70} × 10*−3 and the results are
shown into Fig.11. From this figure, it is found that
*λ is not proportional to g*1*/2*_{, but rather that the }
rela-tionship*λ = C1(g*1*/2+ C2) can be deduced, where*
*C1* is a linear function of the limit, and the constant
*C2* *≈ 0.08, which is not of negligible for the studied*
cases. Thus, it may be noted that the space dependence
of the order parameter, induced by a local stress
con-centration, results in an interface width which cannot
be deduced by simply scaling the numerically obtained
results from the parametric study.

5.6 Effect of material properties and load

In the presented model, the coefficients*α0, β0* and*γ*
in the Landau potential Eq. (3) are material dependent,
but they are not related to the elastic parameters, neither
*is the interface energy coefficient g. Instead changes in*
the elastic properties are introduced in the model via the
shift in the transition temperature as seen in Eq. (15)
and the value of *β, cf. Eq. (*12). The strength of the
interaction between the displacement field and the field
parameter represented by*ξ also affects the evolution of*
a precipitate. For a stiffer material (larger*Λ), β has a*
lower value than for a more compliant material, which
corresponds to an increased*κ. In the case of β > 0, this*
means that the phase transition mode is still of second
order (see Fig.2) but a higher transition rate is achieved,

cf. Table1. However, if*Λ is reduced such that there*
is change in sign of*β to a negative value, first order*
transitions may be possible. The same argument can be
made for a material with a less pronounced interaction
between the displacement field and the order parameter,
i.e. a lower *ξ. Additionally, if KI* *increases, r0* [see

Eq. (13)] and*ρ0*also increase, which leads to a stronger
influence of the crack on its surrounding area.

In the case of diffusionless phase transformation, the approach in the present work may be useful. If all neces-sary material properties and the stress intensity factor are known, the steady state of the second-phase pre-cipitation can be deduced by using the phase diagram outlined in Fig.2. Size, shape, growth rate, time to com-plete transformation, and to some extent the smooth-ness of the interface, can be thereafter be calculated using the dimensionless results presented in this work.

5.7 Further remarks

The presented work, which includes a full paramet-ric study, allows capturing all different scenarii cor-responding to different combinations of load, phe-nomenological coefficients and material properties in time and space for a phase transformation induced by the presence of a crack in a elastic structure. This type of study is usually omitted in the literature. In addition, the microstructure evolution of a material is traditionally modeled by considering two coupled aspects: the phase kinetics and the mechanical equilibrium, and, usually, they are numerically solved separately e.g.Bair et al. (2017),Ma et al.(2006),Thuinet et al.(2013). Here, an analytical solution for the mechanical equilibrium in plane strain for an elastic structure containing a crack is found through the use of the Irwin’s analytical solutions and is directly incorporated into the TDGL equation as inBoulbitch and Korzhenevskii(2016) in order to account for the presence of a fixed crack-induced stress. Thus, only one equation has to be solved rendering the model time-efficient.

A large number of models in the literature, which are based on phase field theory, and the present one employ a phenomenological Landau potential, which derives from a power series in the order parameter. However, these models are not fully quantitative. This limits the study vis-a-vis the effects of temperature tran-sient and temperature gradient (Shi and Xiao 2015), and our understanding of the meaning of the Landau

coef-ficients. An attempt was made byShi and Xiao(2015) to relate the Landau potential coefficients to physical quantities but the study still lies on several arbitrary simplifying assumptions.

For most engineering materials, the structural changes are accompanied by a concentration re-distribution of species, and coupled evolution laws for structural and concentration order parameters may be the tool to suc-cessfully capture such behaviour.

In the case of hydride forming metals, there is a
lack of some of the necessary material data and the
phase transition kinetics are not fully mapped.
*Never-theless, ab-initio calculations such as reported in*
Ols-son et al.(2014, 2015) may contribute to fill in the
gaps, as well as recently performed experiments, cf.
Maimaitiyili et al.(2015),Maimaitiyili et al.(2016).
Further experiments that are especially designed for
capturing phase transformation induced by a crack, are
recommended.

**6 Summary and conclusions**

A phase field approach is used to investigate the forma-tion of a second phase at the vicinity of a crack tip in an isotropic and linear elastic material. The tempo-spatial evolution of the microstructure is computed by numer-ically solving the TDGL equation. To capture the phase transitions, we use a sixth order Landau potential for a single structural order parameter, which represents the degree of ordering of the crystal structure.

For the considered systems the phase diagram for mean-field thermodynamic equilibrium is derived, clearly showing the existence of possible meta-stable phases and first order transitions, which might not emerge by considering the total energy of the sys-tem and the sys-temporal evolution of the space-dependent field. The driving force for the phase transformation at the crack tip can be attributed to the phase transition temperature being locally shifted as a result of the crack induced stress field, which effectively acts as quench-ing in the crack tip vicinity. Different phase transfor-mation scenarios are simulated by using a wide range of combinations of parameters, which represent vary-ing material properties and stress levels. It is found that close to the crack tip, the driving force is always large enough to induce precipitation within a confined area through a second order transformation. The subsequent evolution pattern depends on the parameter set at hand,

and a shift to first order transition during growth of the precipitate is observed occasionally. However, the presence of any metastable phases cannot be revealed from the calculations.

The complete steady-state solutions, with the excep-tion of the shape of the smooth interface, is found to be accurately predicted by using the mean-field solu-tion for each locasolu-tion. The interface width is found not to scale with the interface gradient energy coeffi-cient because of the inhomogeneous stress field around the crack. Finally, the evolution of the order parame-ter is studied following quenching of the whole mate-rial. It is shown that the formation of the second phase is enhanced by the presence of the crack, despite that the entire system undergoes transformation simultane-ously.

Once the diffusionless phase-transformation model parameters of an applicable material system are known, the presented results will allow to predict the kinetics of precipitations, e.g hydride formation, in the crack-tip vicinity. Thus, this will contribute to the failure risk quantification of structures avoiding the use of expen-sive experiments.

**Acknowledgements** The simulations in this work were
per-formed using computational resources provided by the Swedish
National Infrastructure for Computing (SNIC) at LUNARC,
Lund University. The authors are grateful to professor Ali R.
Massih for many valuable discussions.

**Open Access** This article is distributed under the terms of
the Creative Commons Attribution 4.0 International License
(http://creativecommons.org/licenses/by/4.0/), which permits
unrestricted use, distribution, and reproduction in any medium,
provided you give appropriate credit to the original author(s) and
the source, provide a link to the Creative Commons license, and
indicate if changes were made.

**Appendix: Theoretical analysis of the steady state**
**solutions**

In this paragraph the solutions of Eq. (19) presented in
Eqs. (20) and (21) are discussed depending on the signs
of*α0,β and the positive value of κ. All cases described*
below are illustrated by the graphs showing the
poten-tial*Ψ versus the dimensionless order parameter Φ in*
Fig.12.

The condition for ¯*Φ*_{±}2 to exist allowing the
*forma-tion a second phase is A≤ 1/(4 κ) which corresponds*
to*(ρ0/ρ)*1*/2* *≥ [sgn(α0) − 1/(4κ)]/ cos(θ/2). When*

### Φ

0### Ψ

0 A<0 A=0 A>0**(a)**

### Φ

0### Ψ

0 A<0 A=0*A=3/(16κ)*

*A=1/(4κ)*

*A>1/(4κ)*ΔΨ

**(b)**

**Fig. 12 The Landau potential***Ψ versus the dimensionless order*

parameter**Φ. a β > 0, b β < 0**

this condition is fulfilled several situations for which a second phase may nucleate are possible:

– if *α0* *< 0, which induces A < 0, the value ¯Φ*_{−}
cannot exist for any values of *β. Consequently,*

the three solutions are{−| ¯*Φ+|, 0, | ¯Φ+|} where the*
non-zero solutions minimize the system energy.
Thus, a stable second phase is suppose to form in
every point of the system;

– if*α0> 0, β < 0 and A > 0, i.e. _{ρ}ρ*

0 ≥ cos

2*θ*
2, there
are five solutions:{−| ¯*Φ*_{+}*|, −| ¯Φ*_{−}*|, 0, | ¯Φ*_{−}*|, | ¯Φ*_{+}|}.
Since the equation solving gives 3 minima, two
non-zero and 0, both phases can exist in 2 states:
stable or metastable. The stable phase is designed
by a global minimum and the metastable one
cor-responds to a local minimum. When *Ψ ( ¯Φ) = 0*
together with*δ Ψ ( ¯Φ)/δ ¯Φ = 0 which yields A =*

3

16* _{κ}* all minima are equal, i.e. both phases are
equally stable. For

_{16}3

_{κ}*≤ A ≤*

_{4}1

*then the solid solution is expected to be stable and the second phase to be metastable. If 0*

_{κ}*≤ A ≤*

_{16}3

*then the solid solution is expected to be metastable and the second phase to be stable.*

_{κ}– if*α0> 0, β < 0 and A ≤ 0, i.e. _{ρ}ρ*

0 *< cos*

2*θ*
2, the
solutions of the equation are{−| ¯*Φ+|, 0, | ¯Φ+|}. In*
this situation, both minima induces the formation
of a stable second phase.

– if*α0* *> 0, β > 0 and A ≤ 0, i.e.* _{ρ}ρ

0 ≤ cos

2*θ*
2,
the system has 2 minima,{−| ¯*Φ+|, | ¯Φ+|}, and one*
maximum, 0. In these condition, the stable second
phase is expected to form;

If the system has the configurations*{α0* *> 0, β < 0,*
*A* *>* _{4}1_{κ}} and {α0*> 0, β > 0, A > 0}, the solid*
solution is stable and no second phase is expected to
nucleate.

**References**

Allen RM (1978) A high resolution transmission electron micro-scope study of early stage precipitation on dislocation lines in Al-Zn-Mg. Metall Trans A 9(9):1251–1258

Bair J, Zaeem MA, Schwen D (2017) Formation path of hydrides in zirconium by multiphase field modeling. Acta Mater 123:235–244

Barba-Ortega J, Becerra A, González J (2009) Effect of an columnar defect on vortex configuration in a superconduct-ing mesoscopic sample. Braz J Phys 39:673–676 Berger J (2005) Time-dependent Ginzburg-Landau equations

with charged boundaries. J Math Phys 46(9):095106 Birnbaum H (1976) Second phase embrittlement of solids. Scr

Metall 10(8):747–750

Birnbaum H (1984) Mechanical properties of metal hydrides. J Less Common Met 104(1):31–41

Bjerkén C, Massih AR (2014) Phase ordering kinetics of second-phase formation near an edge dislocation. Philos Mag 94(1):569–593

Boulbitch A, Korzhenevskii AL (2016) Crack velocity jumps engendered by a transformational process zone. Phys Rev E 93:063001

Boulbitch AA, Tolédano P (1998) Phase nucleation of elastic defects in crystals undergoing a phase transition. Phys Rev Lett 81:838–841

Cann C, Sexton E (1980) An electron optical study of hydride precipitation and growth at crack tips in zirconium. Acta Metall 28(9):1215–1221

Cao R, Yang T, Horng L, Wu T (2013) Ginzburg-Landau study of superconductor with regular pinning array. J Supercond Nov Magn 26(5):2027–2031

Chen LQ (2002) Phase-field models for microstructure evolu-tion. Annu Rev Mater Res 32:113

Chen C, Li S, Zheng H, Wang L, Lu K (2004) An investigation on structure, deformation and fracture of hydrides in titanium with a large range of hydrogen contents. Acta Materialia 52(12):3697–3706

Coleman CE (2007) Cracking of hydride-forming metals and alloys. Compr Struct Integr 6:103–161

Coleman CE, Hardie D (1966) The hydrogen embrittlement of
*α-zirconium–a review. J Less Common Met 11(3):168–185*
Coleman C, Grigoriev V, Inozemtsev V, Markelov V, Roth
M, Kim VMY, Ali KL, Chakravartty J, Mizrahi R,
Lal-gudi R (2009) Delayed hydride cracking in Zircaloy fuel
cladding–an IAEA coordinated research programme. Nucl
Eng Technol 41:1–8

Cowley RA (1980) Structural phase transitions I. Landau theory. Adv Phys 29(1):1–110

Cyrot M (1973) Ginzburg-Landau theory for superconductors. Rep Prog Phys 36:103

Desai RC, Kapral R (2009) Dynamics of self-organized and self-assembled structures. Cambridge University Press, Cambridge

Deschamps A, Bréchet Y (1998) Influence of predeformation and ageing of an AlZnMg alloy II. Modeling of precipitation kinetics and yield stress. Acta Mater 47(1):293–305 Eshelby JD (1957) The determination of the elastic field of an

ellipsoidal inclusion, and related problems. Acta Metall 241(1226):376–396

Evans A, Cannon R (1986) Overview no. 48. Acta Metall 34(5):761–800

Gómez-Ramírez R, Pound G (1973) Nucleation of a second solid phase along dislocations. Metall Trans 4(6):1563–1570 Gonçalves WC, Sardella E, Becerra VF (2014) Numerical

solution of the time dependent Ginzburg-Landau equations for mixed (d + s)-wave superconductors. J Math Phys 55(4):041501

Grossbeck M, Birnbaum H (1977) Low temperature hydrogen embrittlement of niobium II–microscopic observations. Acta Metall 25(2):135–147

Guyer JE, Wheeler D, Warren JA (2009) FiPy: partial differenial equations with python. Comput Sci Eng 11:6–15 Hin C, Bréchet Y, Maugis P, Soisson F (2008) Heterogeneous

precipitation on dislocations: effect of the elastic field on precipitate morphology. Philos Mag 88(10):1555–1567 Hohenberg PC, Halperin BI (1977) Theory of dynamic critical

phenomena. Rev Mod Phys 49:435–479

Hutchinson JW (1989) Mechanisms of toughening in ceramics. Theoretical and applied mechanics. Elsevier, Amsterdam, pp 139–144

Jernkvist L (2014) Multi-field modelling of hydride forming metals part II: application to fracture. Comput Mater Sci 85:383–401

Jernkvist L, Massih A (2014) Multi-field modelling of hydride forming metals. Part I: model formulation and validation. Comput Mater Sci 85:363–382

Jones RH (1992) Stress-corrosion cracking: materials perfor-mance and evaluation. ASM international

Landau LD, Lifshitz EM (1980) Statistical physics, vol 1, 3rd edn. Pergamon, Oxford Chapter XIV

Léonard F, Desai RC (1998) Spinodal decomposition and dislocation lines in thin films and bulk materials. Phys Rev B 58:8277–8288

Luo L, Su Y, Guo J, Fu H (2006) Formation of titanium hydride in Ti6Al4V alloy. J Alloys Compd 425(12):140–144 Ma XQ, Shi SQ, Woo CH, Chen LQ (2006) The phase field

model for hydrogen diffusion and*γ -hydride precipitation*
in zirconium under non-uniformly applied stress. Mech
Mater 381–2:3–10

Maimaitiyili T, Blomqvist J, Steuwer A, Bjerkén C, Zanellato O, Blackmur MS, Andrieux J, Ribeiro F (2015) In situ hydrogen loading on zirconium powder. J Synchrotron Radiat 22(4):995–1000

Maimaitiyili T, Steuwer A, Blomqvist J, Bjerkén C, Blackmur
MS, Zanellato O, Andrieux J, Ribeiro F (2016) Observation
of the*δ to ε Zr-hydride transition by in-situ synchrotron*
X-ray diffraction. Cryst Res Technol 51:663–670
Massih AR (2011a) Phase transformation near dislocations and

cracks. Solid State Phenom 172–174:384–389

Massih AR (2011b) Second-phase nucleation on an edge dislocation. Philos Mag 91:3961–3980

Moelans N, Blanpain B, Wollants P (2008) An introduction to phase-field modeling of microstructure evolution. Calphad 32(2):268–294

Northwood DO, Kosasih U (1983) Hydrides and delayed hydrogen cracking in zirconium and its alloys. Int Met Rev 28(1):92–121

Ohta T (1990) Interface dynamics under the elastic field. J Phys Condens Matter 2:9685–9689

Olsson PAT, Massih AR, Blomqvist J, Holston AMA, Bjerkén C (2014) Ab initio thermodynamics of zirconium hydrides and deuterides. Comput Mater Sci 86:211–222

Olsson PAT, Blomqvist J, Bjerkén C, Massih AR (2015) Ab initio thermodynamics investigation of titanium hydrides. Comput Mater Sci 97:263–275

Provatas N, Elder K (2010) Phase-field methods in materials science and engineering, 1st edn. Wiley, Hoboken Shi SQ, Xiao Z (2015) A quantitative phase field model for

hydride precipitation in zirconium alloys: Part I. Develop-ment of quantitative free energy functional. J Nucl Mater 459:323–329

Shih D, Robertson I, Birnbaum H (1988) Hydrogen embrit-tlement of titanium: in situ tem studies. Acta Metall 36(1):111–124

Singh R, Roychowdhury S, Sinha V, Sinha T, De P, Banerjee S (2004) Delayed hydride cracking in Zr2.5Nb pressure tube material: influence of fabrication routes. Mater Sci Eng A 374(12):342–350

Takano S, Suzuki T (1974) An electron-optical study of -hydride and hydrogen embrittlement of vanadium. Acta Metall 22(3):265–274

Thuinet L, Legris A, Zhang L, Ambard A (2013) Mesoscale modeling of coherent zirconium hydride precipitation under an applied stress. J Nucl Mater 438(1):32–40

Varias A, Massih A (2002) Hydride-induced embrittlement and fracture in metals effect of stress and temperature distribution. J Mech Phys Solids 50:1469–1510